Journal Pre-proof Mie Scattering of Phonons by Point Defects in IV-VI Semiconductors PbTe and GeTe Ruiqiang Guo, Sangyeop Lee PII:
To appear in:
Materials Today Physics
Received Date: 19 November 2019 Revised Date:
23 December 2019
Accepted Date: 30 December 2019
Please cite this article as: R. Guo, S. Lee, Mie Scattering of Phonons by Point Defects in IV-VI Semiconductors PbTe and GeTe, Materials Today Physics, https://doi.org/10.1016/ j.mtphys.2020.100177. This is a PDF file of an article that has undergone enhancements after acceptance, such as the addition of a cover page and metadata, and formatting for readability, but it is not yet the definitive version of record. This version will undergo additional copyediting, typesetting and review before it is published in its final form, but we are providing this version to give early visibility of the article. Please note that, during the production process, errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain. © 2020 Elsevier Ltd. All rights reserved.
Ruiqiang Guo: Conceptualization, Software, Investigation, Writing – Original Draft. Sangyeop Lee: Conceptualization, Supervision, Writing – Reviewing and Editing, Funding Acquisition
Scattering rate / f (ps -1)
Tmatrix Born Klemens
10 101 100 10-1 10-2
0.09 THz 180
PbTe 1 Frequency (THz)
Mie Scattering of Phonons by Point Defects in IV-VI Semiconductors PbTe and GeTe
Ruiqiang Guo1 and Sangyeop Lee1,2,*
Department of Mechanical Engineering and Materials Science, University of Pittsburgh, Pittsburgh, Pennsylvania 15261, USA 2
Department of Physics and Astronomy, University of Pittsburgh, Pittsburgh, Pennsylvania 15261, USA
* [email protected]
Abstract Point defects in solids such as vacancy and dopants often cause large thermal resistance. Since the lattice site occupied by a point defect has a much smaller size than phonon wavelengths, the scattering of thermal acoustic phonons by point defects in solids has been widely assumed the Rayleigh scattering type. In contrast to this conventional perception, using an ab initio Green’s function approach, we show that the scattering by point defects in PbTe and GeTe exhibits Mie scattering characterized by a weaker frequency dependence of the scattering rates and highly asymmetric scattering phase functions. These unusual behaviors occur because the strain field induced by a point defect can extend for a long distance much larger than the lattice spacing. Because of the asymmetric scattering phase functions, the widely used relaxation time approximation fails with an error of ~20% at 300K in predicting lattice thermal conductivity when the vacancy fraction is 1%. Our results show that the phonon scattering by point defects in IV-VI semiconductors cannot be described by the simple kinetic theory combined with Rayleigh scattering.
Keywords Mie scattering, point defects, phonon transport, Rayleigh scattering, Green’s function methods, thermoelectric materials
1. Introduction Scattering of waves by the inhomogeneity of the medium is a fundamental process underpinning diverse applications including electromagnetics, optics, and acoustics [1-4]. This is of equal importance for thermal phonons [5-7]. Randomly distributed particles can result in phonon localization through multiple scattering and interference of phonon waves [8,9]. Periodic inclusions in phononic crystals give rise to new vibrational band structures due to Bragg and Mie scatterings [10,11]. The wavedefect interaction is usually assumed elastic and its characteristics dramatically depend on the size of the scattering centers. The elastic scattering of phonons, analogous to that of electromagnetic (EM) waves, falls into three regimes: (i) Rayleigh scattering for the scattering centers much smaller than the phonon wavelength ( d
λ where d and λ are
the diameter of the scattering center and the wavelength, respectively), (ii) Mie scattering for those with comparable size to the wavelength ( d for those much larger than the wavelength ( d
λ ), and (iii) Geometric scattering
λ ) [12,13].
A point defect at a single lattice site possesses the minimum size of a scattering center in solids. Since the wavelengths of thermal phonons are usually many times of the lattice spacing, the scattering of thermal phonons by a point defect is often considered Rayleigh scattering and exhibits very weak scattering strength for low frequency phonons. The Rayleigh scattering is well captured by the models suggested by Klemens  and Tamura , which assume that the change in mass and interatomic force constants (IFCs) by a point defect is limited to a single lattice site. The recently developed ab initio Green’s function approach [16,17] also shows the Rayleigh scattering behavior for strongly bonded materials, such as diamond and BAs [18-24]. In this report, we show that the point defects in IV-VI semiconductors (PbTe and GeTe), unlike the previously studied materials, cause Mie scattering of thermal phonons. The IV-VI semiconductors are widely used for the applications of thermoelectrics and phase change materials where the thermal conductivity is a key parameter for the device figure-of-merit. Particularly, large amounts of vacancies (1~3%) have been often reported even in single crystals of these materials, which can reduce the lattice thermal conductivity by half or more [25-36]. Also, it is common that thermoelectric materials 3
contain large concentrations of substitutional defects (1 to 2%) to achieve an optimal doping level for a large thermoelectric power factor [26-31].
2. Computational method 2.1 Phonon scattering rates by point defects 2.1.1 Green’s function approach When a phonon mode qs ( q and s represent the wavevector and polarization, respectively) is scattered into another phonon mode q′s′ elastically by a point defect, the transition rate can be calculated using the Green’s function approach [16-24]:
2 πΩ q′s′ T+ (ω 2 ) qs δ (ωq2′s′ − ωq2s ) , ωVd
where ω is the angular frequency of phonons, Ω is the unit cell volume, qs is the phonon eigenstate, and Vd is the defect volume. The T matrix is defined as T + = (I - VG 0+ )-1 V ,
where I is the identity matrix, V is the perturbation matrix representing the differences of atomic mass and IFCs induced by the point defect. The G 0+ is the retarded Green’s function of the unperturbed crystal, which is calculated numerically using the tetrahedron approach . In the general case, the perturbation matrix V can be decomposed into V M and V K , which represent the changes of atomic mass and interatomic force constants (IFCs), respectively. The V M is expressed as
VM = −
M i′ − M i 2 ω , Mi
where M i and Mi′ are the atomic masses at the lattice site i in the perfect and defected crystals, respectively. The V K is constructed based on the IFCs of the perfect ( K ) and defected ( K ′ ) structures, with each matrix element calculated by ViαK , jβ =
Ki′α , j β − K iα , jβ ( M i M j )1/2
where α and β are Cartesian axes, M i and M j represent the pristine atomic masses at lattice sites i and j, respectively. The perturbation matrix consists of only V K for a vacancy but both V K and V M for substitutional defects. 4
Assuming the scattering of phonons by a point defect is independent of other point defects, the phonon-defect scattering rate is 1
= f ∑ Γ qd s,q ′s′ ,
q ′s ′
where f is the volumetric fraction of point defects.
2.1.2 Born approximation and Klemens’ model using realistic phonon dispersion For weak perturbations, the above calculation can be simplified using the Born approximation, i.e., substituting the T matrix in Eq. (1) with the perturbation matrix V, which is the first-order approximation of the Born series: T + = V + VG 0+ V + VG 0+ VG 0+ V + ... ≈ V .
Klemens suggested a simple model for the rate of phonon-vacancy scattering based on the Debye phonon dispersion and an effective mass variance (∆M / M ) 2 = 9 . In order to employ the realistic phonon dispersion from ab initio calculation, we combine the Klemens’ effective mass variance with the Tamura’s model for phononisotope scattering:
τ qisos with
∑∑ g (i) e q′s′
(i ) ⋅ eq′s′ (i ) δ (ωqs − ωq′s′ ) ,
f b (i )[1 − M b (i) / M (i)]2 where fb (i ) and Mb (i) are the fraction and mass of the bth
isotope of atom i, and M (i) is the average mass of the ith atom in the unit cell. In this work, the Klemens’ model for vacancy cases refers to the Eq. (7) with the Klemens’ effective mass variance for g(i) .
2.2 Density functional theory (DFT) calculation We determined the harmonic and anharmonic IFCs from DFT calculations using the projector augmented wave method , as implemented in the Vienna ab initio simulation package (VASP) . The Perdew-Burke-Ernzerhof (PBE) generalized gradient approximation was used for the exchange-correlation functional for all materials . In Table S1, we list the cutoff energy and k-point sampling grid for electronic states used in the relaxation of the primitive cell, as well as the relaxed lattice constants. Also, the spin-orbit interaction was included for the heavy elements Pb and Te. The selfconsistent calculation was performed with the force convergence criteria of 10-6 eV/ Å. 5
The harmonic and anharmonic IFCs were calculated using a supercell of 4×4×4 for Si and a relatively larger one (5×5×5) for PbTe and GeTe in which the long-range interatomic interactions are expected. We test the convergence of IFCs with respect to supercell size, as shown in Fig. S1 in the Supplementary Material.
2.3 Lattice thermal conductivity We calculated the lattice thermal conductivity using two different methods: full matrix and RTA. For the full matrix case, we obtain the total scattering matrix by adding phonon-phonon, phonon-isotope, and phonon-vacancy scattering matrices. For the RTA case, only diagonal terms from the phonon-vacancy scattering matrix are included while full matrices of phonon-phonon and phonon-isotope scattering are used. Then, the linearized Peierls-Boltzmann transport equation was solved with an iterative manner as implemented in ShengBTE . More technical details can be found in previous publications [42-46]. The sampling grids for phonon states in the first Brillouine zone are listed in Table S1. The isotopes of each element are assumed naturally occurring case. Recent studies show that the phonon renormalization and four-phonon scattering are important for predicting thermal properties of materials such as PbTe, particularly at high temperatures [47-51]. As our study focuses on the Mie scattering of phonons by defects, we ignore the phonon renormalization effect and four-phonon scattering for the sake of simplicity.
3. Results and discussion We use an ab initio Green’s function approach to calculate the scattering matrix of phonons by point defects in PbTe (space group Fm3m) and GeTe (R3m) crystals. For comparison, we also present results for Si. The scattering rates were calculated using three different approaches: (i) exact Green’s function calculation based on the T-matrix formalism, (ii) Green’s function calculation to the first order (Born approximation), and (iii) Klemens’ model with the effective mass variance (∆M / M )2 = 9 (the 3M mass difference is derived by considering the removed kinetic and potential energies due to the removal of an atom from the vacancy site) for single vacancy case  combined with Tamura’s formula to consider full phonon dispersion . We call the last approach Klemens’ model in this paper. The T-matrix method and the Born approximation consider mass variance and finite size effects of scattering center by including the changes of IFCs in all nearby atoms, while Klemens’ model assumes an infinitesimally 6
small point defect. Both the Born approximation and Klemens’ model are based on the lowest-order perturbations while the T-matrix method includes all high-order terms. Recent ab initio Green’s function calculations show the failure of the lowest-order perturbative approaches for some strongly bonded materials [18-24]. The calculated phonon-vacancy scattering rates for PbTe, GeTe, and Si are shown in Fig. 1. The Born approximation gives similar results to the T-matrix for PbTe and GeTe, while it severely underestimates the scattering rate for Si. This is due to the relatively small perturbations resulting from the weaker bonding in PbTe and GeTe, making the high-order terms in Eq. (6) become less important compared to the case of Si. Illustrating this, the Frobenius norm of self-interaction IFCs for PbTe (Pb site, 3.76 eV/Å2) and GeTe (Ge site, 5.96 eV/Å2) are much smaller than that for Si (22.23 eV/Å2). It is more noteworthy that the frequency dependence of scattering rates of PbTe and GeTe is much different from that of Si. In general, the phonon scattering by defects follows the Rayleigh scattering in the long wavelength limit and the Mie scattering in the short wavelength limit. The Rayleigh scattering model, combined with the density-ofstates varying with ω 2 in the long wavelength where ω is a phonon frequency, results in the typical ω 4 dependence of phonon-vacancy scattering rates. For Si in Fig. 1, this ω 4 dependence at the low frequency range is well captured by all the three approaches. However, for PbTe and GeTe in the same figure, the scattering rates from the T-matrix and Born approximation show substantially weaker frequency dependence ( ω 2.5 and ω 3 , respectively) down to 0.1 THz. These results show that the phonon-vacancy scattering in PbTe and GeTe is better described by the Mie scattering rather than the Rayleigh scattering in the full phonon spectrum above at least 0.1 THz.
Fig. 1. Phonon-vacancy scattering rates normalized by the atomic fraction of vacancy for (a) PbTe (Pb vacancy), (b) GeTe (Ge vacancy) and (c) Si using three different approaches: T-matrix, Born approximation, and Klemens’ model.
Considering that the phonon wavelength corresponding to 0.1 THz (78.8 Å for the transverse acoustic phonon in PbTe) is much larger than the lattice spacing (3.29 Å for PbTe), our observation of the Mie scattering implies that long-range strain field near the vacancy site is more important for phonon scattering in PbTe and GeTe than the vacancy site itself. We evaluate how far the strain field induced by a single vacancy can persist in these materials. We calculated the Frobenius norm of changes in the self-interaction IFCs for each atom i, || Vii || where Vii is the change of the self-interaction IFC tensor, which reflects the overall change of the IFCs and strain field on atom i . Fig. 2(a) shows the
|| Vii || normalized by || V00 || (where 0 denotes the vacancy site) with respect to the distance between the atom i and the vacancy site. All three materials exhibit || Vii || rapidly decreasing for the first two nearest neighbors. Beyond the second nearest neighbors, PbTe and GeTe still have a significantly large || Vii || as marked by red circles while the || Vii || of Si is close to zero. Similarly, the calculated displacement of equilibrium position of atoms also indicates long-ranged strain field in PbTe and GeTe, as shown in Fig. S2 in the Supplementary Material. The long-ranged strain field induced by a single vacancy in both materials is consistent with the long-ranged interatomic interactions shown in Fig. 2(b) that were previously reported for perfect crystalline phase . This long-range interaction is due to resonance or hybridization between different electronic configurations, i.e., the unsaturated covalent bonding by p-electrons for rocksalt-like crystals . From Fig. 2(a), the changes of IFCs from the vacancy site still exist in the distance of ~ 10 Å, resulting in the strain field with a diameter of at least 20 Å. Thus, thermal phonons with comparable wavelengths experience Mie scattering rather than Rayleigh scattering. This can explain the weaker frequency dependence of phononvacancy scattering for those materials shown in Figs. 1(a) and 1(b). In contrast, the 4 || Vii || in Si is short-ranged, resulting in the ω dependence of the Rayleigh scattering in
Fig. 1(c). 8
Fig. 2. Interatomic force constants showing the long-ranged interaction in PbTe and GeTe: (a) Frobenius norm of the change in self-interaction IFCs as a function of distance from the vacancy for PbTe (Pb vacancy), GeTe (Ge vacancy), and Si. (b) Frobenius norm of IFCs in perfect crystals as a function of the interatomic distance measured from Pb site for PbTe and Ge site for GeTe. Note that all the values of || Vii || and || Kij || are normalized by its maximum at d=0. The plots are shifted along y-direction and the red dashed lines represent y=0. The y-axes are in linear scale.
A notable feature of Mie scattering of EM waves by a particle is the Mie resonance when the diameter of the particle is an integral multiple of the incident EM wavelength. For our case of phonon scattering in PbTe and GeTe, however, we observe no periodic peaks in the scattering rate versus the wavelength of incident phonons for all three acoustic branches as shown in Fig. 3. The Mie resonant scattering does not exist in our case because the strain field smears out in space and its spatial size cannot be explicitly defined. Another characteristic of Mie scattering that further distinguishes it from Rayleigh scattering can be found in the scattering phase function, which describes the angular probability distribution of phonon states after scattering from a given incident phonon [2,53,54]. The scattering phase function is typically plotted in a closed shape, with the distance of each point from the center representing the relative likehood of scattering into that particular direction. Mie scattering usually exhibits a highly asymmetric phase function with forward scattering being more significant than backward scattering, while 9
the phase function of Rayleigh scattering is symmetric . Fig. 4 shows the calculated scattering phase functions where the incident phonon is from the TA1 branch and the phonon states after scattering remain in the TA1 branch. Indeed, when the wavelength is even twelve times of the lattice constant a, the scattering phase functions for PbTe and GeTe are highly asymmetric, while it is symmetric for Si for the same wavelength. As the wavelength decreases, the scattering phase function becomes more asymmetric for all materials. However, for Si, the asymmetry exists only at very short wavelength (≤ ~2a). This behavior is not limited to the TA1-to-TA1 scattering channel shown in Fig. 4 but also exists for all the other acoustic-to-acoustic scattering channels. The scattering phase functions for TA1-to-LA and LA-to-LA are shown in Fig. S3 and S4 in the Supplementary Material. These observations indicate that the strain field is much more important contributor to phonon scattering than a local empty site in PbTe and GeTe. The strain field induced by a point defect in these materials is spatially extended to cause the Mie scattering rather than the Rayleigh scattering down to 0.1 THz. This is similar to the Mie scattering of phonons by a finite-size nanoparticle inclusion [53-56]. Rayleigh scattering therefore can only happen at lower frequencies or longer wavelengths, e.g., < 0.1 THz for the TA branch of PbTe, as shown in Fig. S5 in the Supplementary Material.
Fig. 3. Phonon-vacancy scattering rates normalized by the atomic fraction of vacancy as a function of phonon wavelength for (a) PbTe (Pb vacancy) and (b) GeTe (Ge vacancy) along the Γ-X direction. The scattering rates are calculated by the T-matrix approach. The TA1 refers to low-lying transverse acoustic branch and LA refers to longitudinal acoustic branch.
Fig. 4. Scattering phase functions by a vacancy in PbTe (Pb vacancy), GeTe (Ge vacancy), and Si, where phonon states before and after are in the TA1 branch. The incident phonon along the  direction has an incident angle of 0 degree and a wavelength of twelve, six, and two times of the lattice constant a for each material, respectively.
The asymmetric scattering phase function shows that phonon transport cannot be described with the simple kinetic theory of phonon gas that assumes each scattering 12
process attempts to relax the phonon distribution into the symmetric equilibrium distribution as in the commonly used relaxation time approximation (RTA). The RTA is exact when the scattering phase function is symmetric as shown in the Supplementary Material; all off-diagonal elements of a scattering matrix are canceled out and thus the relaxation of phonons at a certain mode can be described independently from other modes. However, when the scattering phase function is asymmetric, the off-diagonal elements of a scattering matrix become important and thus the relaxation of phonons at a certain mode is coupled to other modes. A similar behavior has been shown in the high thermal conductivity materials where normal phonon-phonon scattering is much stronger than umklapp phonon-phonon scattering; the strong normal scattering results in the asymmetric scattering phase function due to the phonon momentum conservation . In Fig. 5, we calculate the lattice thermal conductivity values κL of PbTe, GeTe, and Si with vacancy using RTA and full scattering matrix. We choose a specific vacancy fraction that reduces κL by ~50% at 300 K such that the phonon-vacancy scattering is comparable to the phonon-phonon scattering in terms of the strength for each material. The vacancy fraction for GeTe and PbTe is 1%, which is practically relevant as many previous studies report this vacancy level even for single crystals [25,34,35]. Fig. 5 shows that the RTA for the phonon-vacancy scattering substantially underestimates κL of PbTe and GeTe but produces almost identical results as the full scattering matrix for Si. At 300 K, the RTA underestimates κL by 15 to 20% for PbTe and GeTe when the vacancy fraction is 1%.
Fig. 5. Temperature dependent lattice thermal conductivity of (a) PbTe, (b) GeTe (trigonal direction), and (c) Si. The f is atomic vacancy fraction. For the RTA case, only diagonal terms of phonon-vacancy scattering matrix are included while the full matrix case includes all elements of the scattering matrix. The phonon-phonon scattering for both cases is included with a full matrix. The thermal conductivity of GeTe along the binary direction is similar to the trigonal direction case and is shown in Fig. S6 in the Supplementary Material.
We further analyze the effects of Mie scattering on phonon spectral thermal conductivity. In Fig. 6, we show the spectral thermal conductivity contribution calculated by RTA and full scattering matrix, providing a simple measure of asymmetricity of scattering phase function and the extent of Mie scattering in the phonon frequency space. From Fig. 6, the RTA and full scattering matrix solutions for PbTe and GeTe show a noticeable difference in a wide range of phonon spectrum, indicating that the Mie scattering is a better description than the Rayleigh scattering in those materials for the wide range of phonon spectrum. This is consistent with the observations in scattering phase functions. Fig. 4 shows that the scattering phase function of PbTe and GeTe is asymmetric at very low phonon frequencies for thermal transport (0.09 THz for PbTe and 0.27 THz for GeTe) and become even more asymmetric as the frequency increases. However, the marked difference between the RTA and full scattering matrix solutions for Si exists only around 5 THz and 12 THz which correspond to the near zone boundary states of transverse and longitudinal acoustic phonons, respectively, where Mie scattering occurs due to extremely short phonon wavelengths. Most phonon states contributing to thermal transport experience the Rayleigh scattering in Si.
Fig. 6. Spectral lattice thermal conductivity of (a) PbTe, (b) GeTe (trigonal direction), and (c) Si, calculated by the full matrix and RTA at 300 K. The f is atomic vacancy fraction.
The Mie scattering behavior is not limited to phonon-vacancy scattering, but also can be observed in phonon-dopant scattering. In Fig. 7, we present the scattering rates of phonons by two widely used dopants for PbTe, Na, and Bi substituting Pb [27-29]. The atomic fraction of dopants is usually high ranging from 1 to 2% for high thermoelectric figure-of-merits [27-29] and therefore its impact on the phonon scattering and lattice thermal conductivity can be significant. Fig. 7 shows that the scattering rate has much weaker frequency dependence than ω 4 , indicating Mie scattering by Na and Bi dopants similar to the Pb vacancy case we have discussed. Also, the scattering phase function shown in Fig. S7 in the Supplementary Material is highly asymmetric for both dopants, confirming the simple kinetic theory can significantly overestimate the thermal resistance by dopants.
Fig. 7. Comparison of phonon scattering rates by Pb vacancy (vPb), Na and Bi substitution for Pb in PbTe from the T-matrix approach. The scattering rates are normalized by the atomic fraction of point defects.
4. Conclusion 15
In summary, we have applied an ab initio Green’s function approach to investigate the scattering of phonons by point defects in PbTe, GeTe, compared to Si. In contrast to the often assumed Rayleigh scattering, the scattering of most acoustic phonons in PbTe and GeTe exhibits Mie scattering behaviors due to the long-ranged strain field induced by point defects. Specifically, the frequency dependence of scattering rates is weaker than the
ω 4 of Rayleigh scattering and the scattering phase function is highly
asymmetric. The latter results in the failure of the relaxation time approximation, with an error of ~20% in predicting the lattice thermal conductivity at 300 K when the vacancy fraction is 1%. Our results highlight the importance of the long-ranged strain field induced by point defects for thermal transport. Similar behavior is expected in other materials with high electronic polarizability (such as IV–VI, V2–VI3, and elemental V materials) and common ferroelectric materials (such as perovskite oxides), which can lead to the long-ranged strain field by a point defect. The significant Mie scattering behavior shows the complexity of phonon scattering by point defects in IV-VI semiconductors, which cannot be described by the simple kinetic theory combined with the conventional Rayleigh scattering.
Acknowledgements We thank Nebil A. Katcho and Lucas Lindsay for helpful discussions. We acknowledge support from National Science Foundation (Award No. 1705756 and 1709307). This work used the Extreme Science and Engineering Discovery Environment (XSEDE) Linux cluster at the Pittsburgh Supercomputing Center through Allocation No. TG-CTS180043 and the Linux cluster of the Center for Research Computing at the University of Pittsburgh.
Appendix A. Supplementary data Supplementary data to this article can be found online at.
References  L. Tsang, J.A. Kong, K.H. Ding, Scattering of electromagnetic waves: Theories and Applications, John Wiley & Sons 2004.  C.F. Bohren, D.R. Huffman, Absorption and scattering of light by small particles, John Wiley & Sons 2008.  M. Kerker, The scattering of light and other electromagnetic radiation: physical chemistry: a series of monographs, Academic press 2013.  G. Kristensson, Scattering of Electromagnetic Waves by Obstacles, The Institution of Engineering and Technology 2016.  J.M. Ziman, Electrons and phonons: the theory of transport phenomena in solids, Oxford University Press 1960.  G. Chen, Nanoscale energy transport and conversion: a parallel treatment of electrons, molecules, phonons, and photons, Oxford University Press 2005.  D.G. Cahill, P.V. Braun, G. Chen, D.R. Clarke, S. Fan, K.E. Goodson, et al. Nanoscale thermal transport. II. 2003–2012, Appl. Phys. Rev. 1 (2014) 011305.  P. Sheng, Introduction to wave scattering, localization and mesoscopic phenomena, Springer 2006.  M.N. Luckyanova, J. Mendoza, H. Lu, B. Song, S. Huang, J. Zhou, et al. Phonon localization in heat conduction, Sci. Adv. 4 (2018) eaat9460.  M. Lu, L. Feng, Y. Chen. Phononic crystals and acoustic metamaterials, Mater. Today. 12 (2009) 34-42.  M. Maldovan. Sound and heat revolutions in phononics, Nature. 503 (2013) 209-217.  D. Walton. Scattering of phonons by a square-well potential and the effect of colloids on the thermal conductivity. I. Experimental, Phys. Rev. 157 (1967) 720.  A. Majumdar. Microscale heat conduction in dielectric thin films, J. Heat Transfer. 115 (1993) 7-16.  P. Klemens. The scattering of low-frequency lattice waves by static imperfections, Proc. Phys. Soc. Sec. A. 68 (1955) 1113.  S. Tamura. Isotope scattering of dispersive phonons in Ge, Phys. Rev. B. 27 (1983) 858.  N. Mingo, K. Esfarjani, D. Broido, D. Stewart. Cluster scattering effects on phonon conduction in graphene, Phys. Rev. B. 81 (2010) 045408.
 A. Kundu, N. Mingo, D.A. Broido, D.A. Stewart. Role of light and heavy embedded nanoparticles on the thermal conductivity of SiGe alloys, Phys.Rev.B. 84 (2011) 125426.  R. Stern, T. Wang, J. Carrete, N. Mingo, G.K. Madsen. Influence of point defects on the thermal conductivity in FeSi, Phys. Rev. B. 97 (2018) 195201.  A. Katre, J. Carrete, T. Wang, G.K.H. Madsen, N. Mingo. Phonon transport unveils the prevalent point defects in GaN, Phys.Rev.Mater. 2 (2018) 050602.  C.A. Polanco, L. Lindsay. Thermal conductivity of InN with point defects from first principles, Phys. Rev. B. 98 (2018) 014306.  C.A. Polanco, L. Lindsay. Ab initio phonon point defect scattering and thermal transport in graphene, Phys. Rev. B. 97 (2018) 014303.  A. Katre, J. Carrete, B. Dongre, G.K. Madsen, N. Mingo. Exceptionally strong phonon scattering by B substitution in cubic SiC, Phys.Rev.Lett. 119 (2017) 075902.  N.H. Protik, J. Carrete, N.A. Katcho, N. Mingo, D. Broido. Ab initio study of the effect of vacancies on the thermal conductivity of boron arsenide, Phys. Rev. B. 94 (2016) 045207.  N. Katcho, J. Carrete, W. Li, N. Mingo. Effect of nitrogen and vacancy defects on the thermal conductivity of diamond: An ab initio Green's function approach, Phys. Rev. B. 90 (2014) 094117.  R. Brebrick, E. Gubner. Composition stability limits of PbTe. II, J.Chem.Phys. 36 (1962) 1283-1289.  J.P. Heremans, V. Jovovic, E.S. Toberer, A. Saramat, K. Kurosaki, A. Charoenphakdee, et al. Enhancement of thermoelectric efficiency in PbTe by distortion of the electronic density of states, Science. 321 (2008) 554-557.  Y. Pei, A. LaLonde, S. Iwanaga, G.J. Snyder. High thermoelectric figure of merit in heavy hole dominated PbTe, Energy Environ. Sci. 4 (2011) 2085-2089.  Q. Zhang, T. Sun, F. Cao, M. Li, M. Hong, J. Yuan, et al. Tuning the shape and thermoelectric property of PbTe nanocrystals by bismuth doping, Nanoscale. 2 (2010) 1256-1259.  L. Yang, Z. Chen, M. Hong, L. Wang, D. Kong, L. Huang, et al. n-type Bi-doped PbTe nanocubes with enhanced thermoelectric performance, Nano Energy. 31 (2017) 105-112.  Q. Zhang, F. Cao, W. Liu, K. Lukas, B. Yu, S. Chen, et al. Heavy doping and band engineering by potassium to improve the thermoelectric figure of merit in p-type pbte, pbse, and pbte1–y se y, J.Am.Chem.Soc. 134 (2012) 10031-10038.  K. Biswas, J. He, I.D. Blum, C. Wu, T.P. Hogan, D.N. Seidman, et al. High-performance bulk thermoelectrics with all-scale hierarchical architectures, Nature. 489 (2012) 414-418.
 J. Woolley, P. Nikolic. Some Properties of GeTe PbTe Alloys, J.Electrochem.Soc. 112 (1965) 82-84.  E. Levin, M. Besser, R. Hanus. Electronic and thermal transport in GeTe: A versatile base for thermoelectric materials, J.Appl.Phys. 114 (2013) 083713.  P. Nukala, R. Agarwal, X. Qian, M.H. Jang, S. Dhara, K. Kumar, et al. Direct observation of metal–insulator transition in single-crystalline germanium telluride nanowire memory devices prior to amorphization, Nano Lett. 14 (2014) 2201-2209.  P. Nukala, C. Lin, R. Composto, R. Agarwal. Ultralow-power switching via defect engineering in germanium telluride phase-change memory devices, Nat. Commun. 7 (2016) 10482.  D. Wu, L. Wu, D. He, L. Zhao, W. Li, M. Wu, et al. Direct observation of vast offstoichiometric defects in single crystalline SnSe, Nano Energy. 35 (2017) 321-330.  P. Lambin, J. Vigneron. Computation of crystal Green's functions in the complex-energy plane with the use of the analytical tetrahedron method, Phys. Rev. B. 29 (1984) 3430.  C. Ratsifaritana, P. Klemens. Scattering of phonons by vacancies, Int.J.Thermophys. 8 (1987) 737-750.  P.E. Blochl. Projector Augmented-Wave Method, Phys.Rev.B. 50 (1994) 17953-17979.  G. Kresse, J. Furthmuller. Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set, Phys.Rev.B. 54 (1996) 11169-11186.  J.P. Perdew, K. Burke, M. Ernzerhof. Generalized gradient approximation made simple, Phys.Rev.Lett. 77 (1996) 3865-3868.  W. Li, J. Carrete, N.A. Katcho, N. Mingo. ShengBTE: A solver of the Boltzmann transport equation for phonons, Comput.Phys.Commun. (2014) 1747-1758.  D.A. Broido, M. Malorny, G. Birner, N. Mingo, D.A. Stewart. Intrinsic lattice thermal conductivity of semiconductors from first principles, Appl.Phys.Lett. 91 (2007) 231922.  A. Ward, D. Broido, D.A. Stewart, G. Deinzer. Ab initio theory of the lattice thermal conductivity in diamond, Phys. Rev. B. 80 (2009) 125203.  L. Lindsay, D. Broido, T. Reinecke. Thermal conductivity and large isotope effect in GaN from first principles, Phys.Rev.Lett. 109 (2012) 095901.  R. Guo, X. Wang, B. Huang. Thermal conductivity of skutterudite CoSb3 from first principles: Substitution and nanoengineering effects, Sci. Rep. 5 (2015) 7806.  A. Romero, E. Gross, M. Verstraete, O. Hellman. Thermal conductivity in PbTe from first principles, Phys. Rev. B. 91 (2015) 214310.
 Y. Lu, T. Sun, D. Zhang. Lattice anharmonicity, phonon dispersion, and thermal conductivity of PbTe studied by the phonon quasiparticle approach, Phys. Rev. B. 97 (2018) 174304.  G.A. Ribeiro, L. Paulatto, R. Bianco, I. Errea, F. Mauri, M. Calandra. Strong anharmonicity in the phonon spectra of PbTe and SnTe from first principles, Phys. Rev. B. 97 (2018) 014306.  Y. Xia. Revisiting lattice thermal transport in PbTe: The crucial role of quartic anharmonicity, Appl. Phys. Lett. 113 (2018) 073901.  N.K. Ravichandran, D. Broido. Unified first-principles theory of thermal properties of insulators, Phys. Rev. B. 98 (2018) 085205.  S. Lee, K. Esfarjani, T. Luo, J. Zhou, Z. Tian, G. Chen. Resonant bonding leads to low lattice thermal conductivity, Nat.Commun. 5 (2014) 3525.  R.S. Prasher. Mie scattering theory for phonon transport in particulate media, J. Heat Transfer. 126 (2004) 793-804.  N. Zuckerman, J.R. Lukes. Acoustic phonon scattering from particles embedded in an anisotropic medium: A molecular dynamics study, Phys. Rev. B. 77 (2008) 094302.  C. Ying, R. Truell. Scattering of a plane longitudinal wave by a spherical obstacle in an isotropically elastic solid, J.Appl.Phys. 27 (1956) 1086-1097.  N.G. Einspruch, E. Witterholt, R. Truell. Scattering of a plane transverse wave by a spherical obstacle in an elastic medium, J.Appl.Phys. 31 (1960) 806-818.
Mie scattering of phonons by point defects is predicted for PbTe and GeTe by ab initio Green’s function approach.
Extended strain field induced by long-range interactions accounts for the occurrence of Mie scattering in a broad spectrum down to 0.1 THz.
Mie scattering is featured by a weak frequency dependence of the scattering rates and highly asymmetric scattering phase functions.
The highly asymmetric scattering phase functions lead to the failure of the simple kinetic theory such as the relaxation time approximation.
Declaration of interests ☒ The authors declare that they have no known competing financial interests or personal relationships that could have appeared to influence the work reported in this paper. ☐The authors declare the following financial interests/personal relationships which may be considered as potential competing interests: